Click here to load reader

View

0Download

0

Embed Size (px)

Micromagnetic studies of three-dimensional

pyramidal shell-structures

A Knittel1, M Franchin1, T Fischbacher1, F Nasirpouri3, S

Bending2 and H Fangohr1

1 School of Engineering Sciences, University of Southampton, SO17 1BJ

Southampton, United Kingdom 2 Department of Physics and Astronomy, University of Bath, BA2 7AY, United

Kingdom 3 Department of Materials Engineering, Sahand University of Technology, Tabriz

51335-1996, Iran

E-mail: [email protected]

Abstract. In this article we present a systematic, numerical analysis of the magnetic

properties of pyramidal-shaped core-shell structures in a size range below 400 nm.

These are three dimensional structures consisting of a ferromagnetic shell which is

grown on top of a non-magnetic core. The standard micromagnetic model without the

magnetocrystalline anisotropy term is used to describe the properties of the shell. We

vary the thickness of the shell between the limiting cases of an ultra thin shell and a

conventional pyramid and delineate different stable magnetic configurations. We find

different kinds of single domain states, which predominantly occur at smaller system

sizes. In analogy to equivalent states in thin square films we term these onion, flower,

C, and S state. At larger system sizes we also observe two types of vortex states,

which we refer to as symmetric and asymmetric vortex state. For a classification of

the observed states, we derive a phase diagram which specifies the magnetic ground

state as a function of structure size and shell thickness. The transitions between

different ground states can be understood qualitatively. We address the issue of

metastability by investigating the stability of all occurring configurations for different

shell thicknesses. For selected geometries and directions hysteresis measurements are

analysed and discussed. We observe that the magnetic behaviour changes distinctively

in the limit of ultra-thin shells. The study has been motivated by the recent progress

made in the growth of faceted core-shell structures.

PACS numbers: 75.75.Fk, 75.60.Jk, 75.78.Cd

Submitted to: New J. Phys.

Micromagnetic studies of three-dimensional pyramidal shell-structures 2

1. Introduction

The magnetocrystalline anisotropy of a bulk magnetic material governs its magnetic

behaviour and is therefore key to its technological applicability. However, it is an

intrinsic property of the material and cannot readily be tailored [1]. In contrast, the

magnetic behaviour of a nanomagnet is also largely influenced by the interaction of the

magnetisation with its shape. This dependency provides the possibility of fine-tuning

magnetic properties through shape-manipulation, which in turn requires very precise

growth techniques.

Lithographic methods have been widely used to produce ordered arrays of

nanoelements [2]. The basic idea is to deposit a thin resist layer onto a substrate,

parts of which are then chemically altered by exposing them to radiation. Finally

different techniques are used in order to transfer the generated pattern into an array of

nanoelements. However, these nanoelements are not very well defined along the direction

perpendicular to the original resist layer. In contrast, chemical methods are based on

what is often referred to as ’bottom up’ approach, i.e. the nanoparticles develop from

smaller units. The challenge of fabricating nanoparticles of non-spherical geometry is

therefore to obtain a suitably anisotropic growth. Corresponding research on magnetic

nanoparticles has led to the growth of a wide variety of shapes for hard magnetic iron

compounds [3, 4].

In this work we use the micromagnetic model in the limit of soft magnetic

materials (thus neglecting the magnetocrystalline anisotropy of Nickel) which allows

us to accurately analyse the competition between the exchange and the magnetostatic

contributions of the model. Due to their non-linearity, analytical approaches to solving

the micromagnetic equations are only feasible for highly symmetric geometries, and

even in those cases, cannot address certain phenomena like metastability. Therefore one

usually employs numerical methods like the finite difference (FD) method or the finite

element (FE) method. The disadvantage of numerical results is that they generally give

less physical insight than a corresponding analytical solution. However, micromagnetic

simulations do not only yield the magnetisation but also other important scalar and

vector fields such as energy densities and effective magnetic fields corresponding to the

different energetic contributions. A careful examination of these fields can reveal a lot

about the underlying physical mechanisms.

Micromagnetic studies of fundamental geometries have been mostly carried out for

two-dimensional structures, such as square [5, 6, 7, 8] and circular [9, 10, 8] platelets, and

ferromagnetic cubes [11, 12]. Due to the above mentioned limitations of standard growth

techniques more complex three dimensional nanoelements have been subject to far less

research. Corresponding micromagnetic studies are also more involved as a standard

FD discretization is only accurate for structures of rectangular symmetry [13]. In the

literature one can find micromagnetic investigations on cones [14, 15], pyramids [14],

partially spherical structures [16, 17], tetrahedra and octahedra [18], and hexagonally

shaped islands [19]. Energetic ground states of spherical core-shell structures have been

Micromagnetic studies of three-dimensional pyramidal shell-structures 3

studied analytically by deriving expressions for the micromagnetic energy contributions

[20].

Our article on the study of the magnetic behaviour of soft-magnetic core-shell

pyramids is structured as follows: In section 2 we briefly motivate the research on

core-shell structures and give a summary of corresponding experimental work on the

growth of pyramidal core-shell structures. In section 3 we introduce the model and

details of how it is implemented (3.1), define the geometry (3.2), and explain how the

micromagnetic configurations have been computed over the parameter space of this

study (3.3). Section 4 comprises characterizations of all found remanent configurations

(4.1.1 and 4.1.2) and an analysis of their stability. Furthermore a phase diagram is

presented which delineates the energetic ground states as a function of the geometry-

defining parameters. In section 4.2 the reversal behaviour along selected directions of

the applied fields is analysed. Finally we summarise our findings in section 5.

2. Motivation

As discussed in the introduction, most experimental and theoretical research has been

devoted to the study of two-dimensional structures. This is mainly due to practical

difficulties that arise in the growth of well-defined, three-dimensional samples. In the

context of three dimensional objects, core-shell structures are advantageous for the

following reasons: they reduce the amount of magnetic material used compared to filled

3D objects which, in the case of expensive components, may lead to significant cost

reductions. In addition, the interaction between the core and shell regions may lead to

interesting physical phenomena. For example the core region could consist of a material

which is superconducting below a certain critical field, HC. In this case the core can

exhibit re-entrant superconductivity when the applied magnetic field compensates the

stray fields due to the ferromagnetic shell. Furthermore, superconductivity can exist up

to applied fields well above the bulk critical field of the core due to these effects. On

the other hand, if the core material is non-magnetic (e.g., the magnetic field in the core

region lies above HC), then the magnetic behaviour of the core-shell structure will be

solely governed by the ferromagnetic shell (the situation assumed in this article). The

transition between the two magnetic states of the core-shell structure depends on the

properties of both core and shell materials, and on the geometry of the structure.

The presented work only considers the properties of the ferromagnetic shell. It has

been motivated by corresponding experimental work on the electrochemical growth of

pyramidal core-shell structures with a Silver (Ag) core and a Nickel (Ni) shell (figure

1), which we will briefly describe in the following: For this a two step dual bath method

is used. First, single crystal pyramidal-shaped silver mesostructures are deposited on a

highly ordered pyrolytic graphite (HOPG) working electrode from an aqueous solution

of 100 mM AgNO3 at a pH value between 2 and 2.5. In the process the potential of the

HOPG working electrode is first set to 1 V for 60 seconds, then to 0 V for 10 seconds, and

finally to −10 mV for 30 seconds. The silver deposition occurs during the last stage via

Micromagnetic studies of three-dimensional pyramidal shell-structures 4

Figure 1: Left: Atomic force microscope (AFM) image of a pyramidal core-shell

structure with a Silver core and a Nic